#------------------------------------------------------------------------------
#$Date: 2024-02-04 14:18:02 +0200 (Sun, 04 Feb 2024) $
#$Revision: 289573 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/57/06/1570610.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1570610
loop_
_publ_author_name
'Ren, Zhen'
'Sun, Jun-Jun'
'Xu, Long'
'Luo, Peng'
'Ma, Zi-Wei'
'Li, Si'
'Si, Yu-Bing'
'Dong, Xi-Yan'
'Pan, Fangfang'
_publ_section_title
;
 X-ray-triggered through-space charge transfer and photochromism in silver
 nanoclusters.
;
_journal_issue                   5
_journal_name_full               Nanoscale
_journal_page_first              2662
_journal_page_last               2671
_journal_paper_doi               10.1039/d3nr05409h
_journal_volume                  16
_journal_year                    2024
_chemical_formula_moiety         'C72 H108 Ag14, Cl'
_chemical_formula_sum            'C72 H109 Ag14 Cl O'
_chemical_formula_weight         2536.22
_space_group_crystal_system      trigonal
_space_group_IT_number           148
_space_group_name_Hall           '-R 3'
_space_group_name_H-M_alt        'R -3 :H'
_atom_sites_solution_hydrogens   mixed
_audit_block_doi                 10.5517/ccdc.csd.cc2gp1nw
_audit_creation_date             2023-07-25
_audit_creation_method
;
Olex2 1.5
(compiled 2023.03.06 svn.rbb2c1857 for OlexSys, GUI svn.r6748)
;
_audit_update_record
;
2023-07-25 deposited with the CCDC.	2023-12-28 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   16.3155(3)
_cell_length_b                   16.3155(3)
_cell_length_c                   29.6131(5)
_cell_measurement_reflns_used    3881
_cell_measurement_temperature    200.00(10)
_cell_measurement_theta_max      73.0970
_cell_measurement_theta_min      4.3300
_cell_volume                     6826.8(2)
_computing_cell_refinement       'CrysAlisPro 1.171.39.27b (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.39.27b (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.39.27b (Rigaku OD, 2015)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_temperature      199.99(10)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.956
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω    -12.00  44.00   0.50    0.50    --    0.00  38.00-150.00  112
  2  ω     53.00  85.00   0.50    0.50    --    0.00  38.00-150.00   64
  3  ω     11.00 113.00   0.50    4.50    --   95.80 -82.00 150.00  204
  4  ω    115.00 171.00   0.50    4.50    --   95.80  45.00 -60.00  112
  5  ω     26.00 119.00   0.50    4.50    --   95.80 -61.00 150.00  186
  6  ω     83.00 134.00   0.50    4.50    --   95.80  45.00 -30.00  102
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB AFC12 (RINC): Kappa single'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0282
_diffrn_reflns_av_unetI/netI     0.0330
_diffrn_reflns_Laue_measured_fraction_full 0.993
_diffrn_reflns_Laue_measured_fraction_max 0.956
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       35
_diffrn_reflns_limit_l_min       -33
_diffrn_reflns_number            6732
_diffrn_reflns_point_group_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.956
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         74.288
_diffrn_reflns_theta_min         3.466
_exptl_absorpt_coefficient_mu    24.077
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.09778
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.39.27b (Rigaku Oxford Diffraction, 2015)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            violet
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    1.851
_exptl_crystal_description       rhombohedral
_exptl_crystal_F_000             3672
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.2
_refine_diff_density_max         0.959
_refine_diff_density_min         -1.011
_refine_diff_density_rms         0.119
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.064
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     219
_refine_ls_number_reflns         2964
_refine_ls_number_restraints     167
_refine_ls_restrained_S_all      1.091
_refine_ls_R_factor_all          0.0559
_refine_ls_R_factor_gt           0.0495
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0838P)²+20.3275P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1393
_refine_ls_wR_factor_ref         0.1438
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2482
_reflns_number_total             2964
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d3nr05409h2.cif
_cod_data_source_block           cl@ag14-cu-ray_sq
_cod_depositor_comments
'Adding full bibliography for 1570610--1570618.cif.'
_cod_original_cell_volume        6826.8(3)
_cod_original_sg_symbol_H-M      'R -3'
_cod_database_code               1570610
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.086
_shelx_estimated_absorpt_t_min   0.065
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.5 times of:
  All C(H,H,H) groups
2. Restrained distances
 C5A-C3 = C4A-C3 = C6A-C3 = C11A-C9A = C10A-C9A = C12A-C9A
 1.53 with sigma of 0.01
 C9-C11 = C9-C10 = C9-C12 = C6-C3 = C5-C3 = C4-C3
 1.53 with sigma of 0.01
 C8A-C9A = C9-C8
 1.5 with sigma of 0.02
 C4A-C5A \\sim C4A-C6A \\sim C5A-C6A \\sim C11A-C12A \\sim C12A-C10A \\sim
C10A-C11A
 with sigma of 0.02
 C10-C11 \\sim C10-C12 \\sim C11-C12 \\sim C4-C5 \\sim C4-C6 \\sim C5-C6
 with sigma of 0.02
3. Uiso/Uaniso restraints and constraints
Uanis(C4A) \\sim Ueq, Uanis(C5A) \\sim Ueq, Uanis(C6A) \\sim Ueq, Uanis(C7A)
\\sim Ueq, Uanis(C8A) \\sim Ueq, Uanis(C9A) \\sim Ueq, Uanis(C10A) \\sim Ueq,
Uanis(C11A) \\sim Ueq, Uanis(C12A) \\sim Ueq: with sigma of 0.01 and sigma for
terminal atoms of 0.02
Uanis(C3) \\sim Ueq, Uanis(C4) \\sim Ueq, Uanis(C5) \\sim Ueq, Uanis(C6) \\sim
Ueq, Uanis(C7) \\sim Ueq, Uanis(C8) \\sim Ueq, Uanis(C9) \\sim Ueq, Uanis(C10)
\\sim Ueq, Uanis(C11) \\sim Ueq, Uanis(C12) \\sim Ueq: with sigma of 0.01 and
sigma for terminal atoms of 0.02
Uanis(Ag3) = Uanis(Ag3A)
Uanis(C7A) = Uanis(C7)
4. Rigid body (RIGU) restrains
 C4A, C3, C6
 with sigma for 1-2 distances of 0.0001 and sigma for 1-3 distances of 0.0001
 C9, C12
 with sigma for 1-2 distances of 0.0001 and sigma for 1-3 distances of 0.0001
5. Others
 Sof(Ag3A)=1-FVAR(1)
 Sof(Ag3)=FVAR(1)
 Sof(C4A)=Sof(H4AA)=Sof(H4AB)=Sof(H4AC)=Sof(C5A)=Sof(H5AA)=Sof(H5AB)=Sof(H5AC)=
 Sof(C6A)=Sof(H6AA)=Sof(H6AB)=Sof(H6AC)=1-FVAR(2)
 Sof(C4)=Sof(H4A)=Sof(H4B)=Sof(H4C)=Sof(C5)=Sof(H5A)=Sof(H5B)=Sof(H5C)=Sof(C6)=
 Sof(H6A)=Sof(H6B)=Sof(H6C)=FVAR(2)
 Sof(C7A)=Sof(C8A)=Sof(C9A)=Sof(C10A)=Sof(H10D)=Sof(H10E)=Sof(H10F)=Sof(C11A)=
 Sof(H11D)=Sof(H11E)=Sof(H11F)=Sof(C12A)=Sof(H12D)=Sof(H12E)=Sof(H12F)=1-FVAR(3)
 Sof(C7)=Sof(C8)=Sof(C9)=Sof(C10)=Sof(H10A)=Sof(H10B)=Sof(H10C)=Sof(C11)=
 Sof(H11A)=Sof(H11B)=Sof(H11C)=Sof(C12)=Sof(H12A)=Sof(H12B)=Sof(H12C)=FVAR(3)
6.a Riding coordinates:
 C4(H4A,H4B,H4C), C5(H5A,H5B,H5C), C6(H6A,H6B,H6C), C4A(H4AA,H4AB,H4AC),
 C10A(H10D,H10E,H10F), C11A(H11D,H11E,H11F)
6.b Idealised Me refined as rotating group:
 C10(H10A,H10B,H10C), C11(H11A,H11B,H11C), C12(H12A,H12B,H12C), C5A(H5AA,H5AB,
 H5AC), C6A(H6AA,H6AB,H6AC), C12A(H12D,H12E,H12F)
;
_smtbx_masks_special_details
;
A solvent mask was calculated and 225 electrons were 
found in a volume of 783Å³ in 2 voids per unit cell. 
This is consistent with the presence of 
3[OH] and 10[CH3OH] per Unit Cell 
which account for 207 electrons 
per unit cell.
;
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ag1 Ag 0.47968(4) 0.63561(4) 0.60322(2) 0.0708(2) Uani 1 1 d . . . . .
Ag2 Ag 0.333333 0.666667 0.56207(3) 0.0731(3) Uani 1 3 d S T P A .
Cl1 Cl 0.333333 0.666667 0.666667 0.0443(5) Uani 1 6 d S T P . .
C1 C 0.4634(5) 0.5238(5) 0.6427(2) 0.0683(15) Uani 1 1 d . . . . .
C2 C 0.4725(6) 0.4644(6) 0.6611(3) 0.082(2) Uani 1 1 d . . . . .
C3 C 0.4859(8) 0.3898(8) 0.6820(4) 0.131(3) Uani 1 1 d D U . . .
Ag3 Ag 0.52445(11) 0.82691(8) 0.63107(3) 0.0684(3) Uani 0.836(4) 1 d . . P A 1
C4 C 0.511(2) 0.342(2) 0.6444(8) 0.165(12) Uani 0.469(17) 1 d D U P B 1
H4A H 0.487451 0.352397 0.616558 0.248 Uiso 0.469(17) 1 d R U P B 1
H4B H 0.484611 0.275187 0.649078 0.248 Uiso 0.469(17) 1 d R U P B 1
H4C H 0.578771 0.371807 0.642928 0.248 Uiso 0.469(17) 1 d R U P B 1
C5 C 0.4015(15) 0.3205(16) 0.7096(9) 0.135(9) Uani 0.469(17) 1 d D U P B 1
H5A H 0.401704 0.332318 0.741363 0.203 Uiso 0.469(17) 1 d R U P B 1
H5B H 0.390994 0.257668 0.705063 0.203 Uiso 0.469(17) 1 d R U P B 1
H5C H 0.351914 0.326218 0.695183 0.203 Uiso 0.469(17) 1 d R U P B 1
C6 C 0.5735(17) 0.449(2) 0.7119(10) 0.187(9) Uani 0.469(17) 1 d D U P B 1
H6A H 0.574613 0.404438 0.732524 0.280 Uiso 0.469(17) 1 d R U P B 1
H6B H 0.556713 0.489918 0.727864 0.280 Uiso 0.469(17) 1 d R U P B 1
H6C H 0.634943 0.486538 0.698544 0.280 Uiso 0.469(17) 1 d R U P B 1
C7 C 0.4920(12) 0.7390(12) 0.5583(6) 0.061(3) Uani 0.62(2) 1 d . U P A 1
C8 C 0.5166(13) 0.7956(13) 0.5288(5) 0.080(4) Uani 0.62(2) 1 d D U P A 1
C9 C 0.5455(12) 0.8601(12) 0.4885(5) 0.123(6) Uani 0.62(2) 1 d D U P A 1
C10 C 0.580(2) 0.8165(17) 0.4525(7) 0.191(12) Uani 0.62(2) 1 d D U P A 1
H10A H 0.625239 0.801228 0.465891 0.287 Uiso 0.62(2) 1 calc R U P A 1
H10B H 0.609887 0.861770 0.427757 0.287 Uiso 0.62(2) 1 calc R U P A 1
H10C H 0.525384 0.758583 0.440705 0.287 Uiso 0.62(2) 1 calc R U P A 1
C11 C 0.4588(15) 0.8647(18) 0.4729(8) 0.193(12) Uani 0.62(2) 1 d D U P A 1
H11A H 0.413698 0.804677 0.458550 0.290 Uiso 0.62(2) 1 calc R U P A 1
H11B H 0.478248 0.916395 0.451064 0.290 Uiso 0.62(2) 1 calc R U P A 1
H11C H 0.428814 0.876109 0.498924 0.290 Uiso 0.62(2) 1 calc R U P A 1
C12 C 0.6263(15) 0.9571(16) 0.5031(10) 0.182(10) Uani 0.62(2) 1 d D U P A 1
H12A H 0.652507 0.950953 0.531849 0.273 Uiso 0.62(2) 1 calc R U P A 1
H12B H 0.602050 1.000893 0.506834 0.273 Uiso 0.62(2) 1 calc R U P A 1
H12C H 0.675933 0.981636 0.480019 0.273 Uiso 0.62(2) 1 calc R U P A 1
Ag3A Ag 0.5609(5) 0.8496(4) 0.62338(16) 0.0684(3) Uani 0.164(4) 1 d . . P A 2
C4A C 0.4016(16) 0.2948(15) 0.6669(11) 0.211(11) Uani 0.531(17) 1 d D U P B 2
H4AA H 0.416703 0.246078 0.673015 0.317 Uiso 0.531(17) 1 d R U P B 2
H4AB H 0.388263 0.294528 0.635275 0.317 Uiso 0.531(17) 1 d R U P B 2
H4AC H 0.347043 0.283258 0.684155 0.317 Uiso 0.531(17) 1 d R U P B 2
C5A C 0.480(2) 0.3927(19) 0.7338(4) 0.159(11) Uani 0.531(17) 1 d D U P B 2
H5AA H 0.529878 0.454182 0.744958 0.239 Uiso 0.531(17) 1 calc R U P B 2
H5AB H 0.488292 0.342229 0.747006 0.239 Uiso 0.531(17) 1 calc R U P B 2
H5AC H 0.418006 0.383574 0.742546 0.239 Uiso 0.531(17) 1 calc R U P B 2
C6A C 0.5761(12) 0.3940(17) 0.6673(8) 0.127(8) Uani 0.531(17) 1 d D U P B 2
H6AA H 0.567695 0.330205 0.667894 0.190 Uiso 0.531(17) 1 calc R U P B 2
H6AB H 0.627364 0.435072 0.687917 0.190 Uiso 0.531(17) 1 calc R U P B 2
H6AC H 0.591977 0.419493 0.636595 0.190 Uiso 0.531(17) 1 calc R U P B 2
C7A C 0.515(2) 0.758(2) 0.5660(10) 0.061(3) Uani 0.38(2) 1 d . U P A 2
C8A C 0.550(2) 0.8174(18) 0.5392(8) 0.077(7) Uani 0.38(2) 1 d D U P A 2
C9A C 0.5878(18) 0.8833(17) 0.5011(8) 0.127(11) Uani 0.38(2) 1 d D U P A 2
C10A C 0.614(3) 0.9788(18) 0.5219(11) 0.157(14) Uani 0.38(2) 1 d D U P A 2
H10D H 0.564514 0.992859 0.515197 0.235 Uiso 0.38(2) 1 d R U P A 2
H10E H 0.672074 1.026269 0.508657 0.235 Uiso 0.38(2) 1 d R U P A 2
H10F H 0.621234 0.978279 0.554057 0.235 Uiso 0.38(2) 1 d R U P A 2
C11A C 0.677(2) 0.885(3) 0.4848(12) 0.162(14) Uani 0.38(2) 1 d D U P A 2
H11D H 0.665446 0.821692 0.479342 0.243 Uiso 0.38(2) 1 d R U P A 2
H11E H 0.723406 0.913492 0.508352 0.243 Uiso 0.38(2) 1 d R U P A 2
H11F H 0.700666 0.921442 0.457632 0.243 Uiso 0.38(2) 1 d R U P A 2
C12A C 0.522(2) 0.864(3) 0.4607(10) 0.154(14) Uani 0.38(2) 1 d D U P A 2
H12D H 0.478181 0.886861 0.467628 0.231 Uiso 0.38(2) 1 calc R U P A 2
H12E H 0.486952 0.796394 0.454517 0.231 Uiso 0.38(2) 1 calc R U P A 2
H12F H 0.560277 0.898101 0.434216 0.231 Uiso 0.38(2) 1 calc R U P A 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0181 0.0091 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag 0.1306 4.2820 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.3639 0.7018 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0492 0.0322 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Ag2 Ag1 Ag3 74.10(2) . . ?
Ag2 Ag1 Ag3A 79.22(10) . . ?
Ag2 Ag1 Ag3A 127.46(11) . 14_456 ?
Ag2 Ag1 Ag3A 77.51(9) . 3_565 ?
C1 Ag1 Ag2 128.96(19) . . ?
C1 Ag1 Ag3 53.94(19) . 3_565 ?
C1 Ag1 Ag3 129.08(19) . . ?
C1 Ag1 Ag3 54.07(19) . 14_456 ?
C1 Ag1 C7 174.5(5) . . ?
C1 Ag1 Ag3A 132.5(2) . . ?
C1 Ag1 Ag3A 51.9(2) . 3_565 ?
C1 Ag1 Ag3A 48.4(2) . 14_456 ?
C1 Ag1 C7A 172.5(9) . . ?
Ag3 Ag1 Ag2 118.80(4) 14_456 . ?
Ag3 Ag1 Ag2 75.03(2) 3_565 . ?
Ag3 Ag1 Ag3 75.03(3) 14_456 . ?
Ag3 Ag1 Ag3 75.97(3) 3_565 14_456 ?
Ag3 Ag1 Ag3 119.00(6) 3_565 . ?
Ag3 Ag1 Ag3A 8.91(10) 14_456 14_456 ?
Ag3 Ag1 Ag3A 80.95(10) . 14_456 ?
Ag3 Ag1 Ag3A 78.18(9) 3_565 14_456 ?
Ag3 Ag1 Ag3A 81.47(10) 14_456 3_565 ?
Ag3 Ag1 Ag3A 127.41(13) . 3_565 ?
Ag3 Ag1 Ag3A 8.63(9) 3_565 3_565 ?
C7 Ag1 Ag2 49.6(5) . . ?
C7 Ag1 Ag3 56.4(5) . . ?
C7 Ag1 Ag3 124.4(5) . 3_565 ?
C7 Ag1 Ag3 131.4(5) . 14_456 ?
C7 Ag1 Ag3A 137.1(5) . 14_456 ?
C7 Ag1 Ag3A 125.5(5) . 3_565 ?
Ag3A Ag1 Ag3A 84.25(11) . 14_456 ?
Ag3A Ag1 Ag3A 82.59(10) 3_565 14_456 ?
C7A Ag1 Ag2 58.4(8) . . ?
C7A Ag1 Ag3 122.6(8) . 14_456 ?
C7A Ag1 Ag3A 127.2(8) . 14_456 ?
C7A Ag1 Ag3A 43.2(8) . . ?
Ag1 Ag2 Ag1 104.04(2) 2_665 . ?
Ag1 Ag2 Ag1 104.04(2) 3_565 . ?
Ag1 Ag2 Ag1 104.04(2) 2_665 3_565 ?
C7 Ag2 Ag1 44.8(5) 2_665 2_665 ?
C7 Ag2 Ag1 85.3(5) 3_565 . ?
C7 Ag2 Ag1 85.3(5) . 2_665 ?
C7 Ag2 Ag1 44.8(5) 3_565 3_565 ?
C7 Ag2 Ag1 44.8(5) . . ?
C7 Ag2 Ag1 148.7(5) 3_565 2_665 ?
C7 Ag2 Ag1 148.7(5) 2_665 . ?
C7 Ag2 Ag1 85.3(5) 2_665 3_565 ?
C7 Ag2 Ag1 148.7(5) . 3_565 ?
C7 Ag2 C7 119.75(8) 2_665 3_565 ?
C7 Ag2 C7 119.75(8) 2_665 . ?
C7 Ag2 C7 119.76(8) 3_565 . ?
C7 Ag2 C7A 6.3(11) 3_565 3_565 ?
C7 Ag2 C7A 123.3(13) 2_665 3_565 ?
C7 Ag2 C7A 116.9(13) 3_565 2_665 ?
C7 Ag2 C7A 116.9(13) . 3_565 ?
C7 Ag2 C7A 6.3(11) 2_665 2_665 ?
C7 Ag2 C7A 123.3(13) . 2_665 ?
C7A Ag2 Ag1 146.5(7) . 3_565 ?
C7A Ag2 Ag1 146.5(7) 2_665 . ?
C7A Ag2 Ag1 80.1(8) 3_565 . ?
C7A Ag2 Ag1 44.1(8) 3_565 3_565 ?
C7A Ag2 Ag1 80.1(8) 2_665 3_565 ?
C7A Ag2 Ag1 146.5(7) 3_565 2_665 ?
C7A Ag2 Ag1 80.1(8) . 2_665 ?
C7A Ag2 Ag1 44.1(8) 2_665 2_665 ?
C7A Ag2 Ag1 44.1(8) . . ?
C7A Ag2 C7A 119.80(11) 2_665 . ?
C7A Ag2 C7A 119.80(11) . 3_565 ?
C7A Ag2 C7A 119.80(11) 2_665 3_565 ?
Ag1 C1 Ag3 81.8(2) . 14_456 ?
Ag1 C1 Ag3 80.9(2) . 3_565 ?
Ag1 C1 Ag3A 92.0(3) . 14_456 ?
Ag1 C1 Ag3A 88.1(3) . 3_565 ?
C2 C1 Ag1 165.5(6) . . ?
C2 C1 Ag3 103.0(6) . 14_456 ?
C2 C1 Ag3 111.6(6) . 3_565 ?
C2 C1 Ag3A 103.0(6) . 3_565 ?
C2 C1 Ag3A 91.0(6) . 14_456 ?
Ag3 C1 Ag3 97.5(2) 3_565 14_456 ?
Ag3 C1 Ag3A 109.1(3) 14_456 3_565 ?
Ag3 C1 Ag3A 13.47(14) 14_456 14_456 ?
Ag3 C1 Ag3A 12.68(13) 3_565 3_565 ?
Ag3 C1 Ag3A 108.0(3) 3_565 14_456 ?
C1 C2 C3 177.3(8) . . ?
C2 C3 C4 107.6(12) . . ?
C2 C3 C5 112.9(11) . . ?
C2 C3 C6 101.3(15) . . ?
C2 C3 C4A 106.4(16) . . ?
C2 C3 C5A 110.8(10) . . ?
C2 C3 C6A 112.7(10) . . ?
C4 C3 C6 109.8(10) . . ?
C5 C3 C4 112.8(11) . . ?
C5 C3 C6 111.8(10) . . ?
C4A C3 C5A 106.4(10) . . ?
C6A C3 C4A 108.9(10) . . ?
C6A C3 C5A 111.2(10) . . ?
Ag1 Ag3 Ag1 104.77(5) 2_665 15_556 ?
Ag1 Ag3 Ag1 105.43(4) 2_665 . ?
Ag1 Ag3 Ag1 103.21(3) 15_556 . ?
C1 Ag3 Ag1 148.41(17) 15_556 2_665 ?
C1 Ag3 Ag1 81.81(16) 15_556 . ?
C1 Ag3 Ag1 149.80(17) 2_665 . ?
C1 Ag3 Ag1 45.16(16) 2_665 2_665 ?
C1 Ag3 Ag1 82.64(17) 2_665 15_556 ?
C1 Ag3 Ag1 44.15(16) 15_556 15_556 ?
C1 Ag3 C1 119.18(10) 2_665 15_556 ?
C1 Ag3 C7 119.7(5) 15_556 . ?
C1 Ag3 C7 121.1(5) 2_665 . ?
C7 Ag3 Ag1 146.2(4) . 15_556 ?
C7 Ag3 Ag1 82.3(5) . 2_665 ?
C7 Ag3 Ag1 43.9(5) . . ?
C3 C4 H4A 107.5 . . ?
C3 C4 H4B 113.0 . . ?
C3 C4 H4C 107.9 . . ?
H4A C4 H4B 109.5 . . ?
H4A C4 H4C 109.5 . . ?
H4B C4 H4C 109.4 . . ?
C3 C5 H5A 117.9 . . ?
C3 C5 H5B 109.4 . . ?
C3 C5 H5C 100.6 . . ?
H5A C5 H5B 109.4 . . ?
H5A C5 H5C 109.5 . . ?
H5B C5 H5C 109.5 . . ?
C3 C6 H6A 104.6 . . ?
C3 C6 H6B 102.9 . . ?
C3 C6 H6C 120.6 . . ?
H6A C6 H6B 109.4 . . ?
H6A C6 H6C 109.5 . . ?
H6B C6 H6C 109.4 . . ?
Ag1 C7 Ag2 85.6(6) . . ?
Ag1 C7 Ag3 79.6(6) . . ?
Ag2 C7 Ag3 96.7(7) . . ?
C8 C7 Ag1 164.1(17) . . ?
C8 C7 Ag2 107.3(14) . . ?
C8 C7 Ag3 107.2(13) . . ?
C7 C8 C9 174.7(19) . . ?
C8 C9 C10 106.8(15) . . ?
C8 C9 C11 107.5(14) . . ?
C8 C9 C12 107.8(17) . . ?
C11 C9 C10 111.8(11) . . ?
C11 C9 C12 112.0(11) . . ?
C12 C9 C10 110.6(11) . . ?
C9 C10 H10A 109.5 . . ?
C9 C10 H10B 109.5 . . ?
C9 C10 H10C 109.5 . . ?
H10A C10 H10B 109.5 . . ?
H10A C10 H10C 109.5 . . ?
H10B C10 H10C 109.5 . . ?
C9 C11 H11A 109.5 . . ?
C9 C11 H11B 109.5 . . ?
C9 C11 H11C 109.5 . . ?
H11A C11 H11B 109.5 . . ?
H11A C11 H11C 109.5 . . ?
H11B C11 H11C 109.5 . . ?
C9 C12 H12A 109.5 . . ?
C9 C12 H12B 109.5 . . ?
C9 C12 H12C 109.5 . . ?
H12A C12 H12B 109.5 . . ?
H12A C12 H12C 109.5 . . ?
H12B C12 H12C 109.5 . . ?
Ag1 Ag3A Ag1 93.07(15) . 15_556 ?
Ag1 Ag3A Ag1 94.22(17) . 2_665 ?
Ag1 Ag3A Ag1 91.13(16) 2_665 15_556 ?
C1 Ag3A Ag1 74.1(2) 2_665 15_556 ?
C1 Ag3A Ag1 130.1(3) 2_665 . ?
C1 Ag3A Ag1 39.61(17) 15_556 15_556 ?
C1 Ag3A Ag1 78.0(2) 15_556 . ?
C1 Ag3A Ag1 128.3(3) 15_556 2_665 ?
C1 Ag3A Ag1 40.02(17) 2_665 2_665 ?
C1 Ag3A C1 111.9(2) 15_556 2_665 ?
C1 Ag3A C8A 110.1(7) 2_665 . ?
C1 Ag3A C8A 137.1(7) 15_556 . ?
C7A Ag3A Ag1 80.5(10) . 2_665 ?
C7A Ag3A Ag1 42.2(9) . . ?
C7A Ag3A C1 118.8(10) . 2_665 ?
C7A Ag3A C8A 27.0(10) . . ?
C8A Ag3A Ag1 81.3(7) . 2_665 ?
C8A Ag3A Ag1 68.4(6) . . ?
C3 C4A H4AA 108.0 . . ?
C3 C4A H4AB 112.0 . . ?
C3 C4A H4AC 108.4 . . ?
H4AA C4A H4AB 109.4 . . ?
H4AA C4A H4AC 109.5 . . ?
H4AB C4A H4AC 109.5 . . ?
C3 C5A H5AA 109.5 . . ?
C3 C5A H5AB 109.5 . . ?
C3 C5A H5AC 109.5 . . ?
H5AA C5A H5AB 109.5 . . ?
H5AA C5A H5AC 109.5 . . ?
H5AB C5A H5AC 109.5 . . ?
C3 C6A H6AA 109.5 . . ?
C3 C6A H6AB 109.5 . . ?
C3 C6A H6AC 109.5 . . ?
H6AA C6A H6AB 109.5 . . ?
H6AA C6A H6AC 109.5 . . ?
H6AB C6A H6AC 109.5 . . ?
Ag1 C7A Ag2 77.5(9) . . ?
Ag1 C7A Ag3A 94.6(12) . . ?
Ag3A C7A Ag2 110.1(14) . . ?
C8A C7A Ag1 160(3) . . ?
C8A C7A Ag2 114(2) . . ?
C8A C7A Ag3A 96(2) . . ?
C7A C8A Ag3A 56.8(18) . . ?
C7A C8A C9A 173(3) . . ?
C9A C8A Ag3A 130.2(18) . . ?
C8A C9A C10A 104(2) . . ?
C8A C9A C11A 107(2) . . ?
C8A C9A C12A 118(2) . . ?
C10A C9A C11A 109.7(13) . . ?
C10A C9A C12A 109.4(13) . . ?
C12A C9A C11A 108.8(12) . . ?
C9A C10A H10D 108.7 . . ?
C9A C10A H10E 108.4 . . ?
C9A C10A H10F 111.3 . . ?
H10D C10A H10E 109.5 . . ?
H10D C10A H10F 109.4 . . ?
H10E C10A H10F 109.5 . . ?
C9A C11A H11D 111.0 . . ?
C9A C11A H11E 106.7 . . ?
C9A C11A H11F 110.6 . . ?
H11D C11A H11E 109.5 . . ?
H11D C11A H11F 109.4 . . ?
H11E C11A H11F 109.5 . . ?
C9A C12A H12D 109.5 . . ?
C9A C12A H12E 109.5 . . ?
C9A C12A H12F 109.5 . . ?
H12D C12A H12E 109.5 . . ?
H12D C12A H12F 109.5 . . ?
H12E C12A H12F 109.5 . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ag1 Ag2 2.9415(6) . ?
Ag1 C1 2.070(7) . ?
Ag1 Ag3 2.9453(9) . ?
Ag1 Ag3 2.8826(11) 3_565 ?
Ag1 Ag3 2.9415(11) 14_456 ?
Ag1 C7 2.078(19) . ?
Ag1 Ag3A 3.244(5) 14_456 ?
Ag1 Ag3A 3.111(5) . ?
Ag1 Ag3A 3.217(6) 3_565 ?
Ag1 C7A 2.10(3) . ?
Ag2 C7 2.248(17) . ?
Ag2 C7 2.248(17) 2_665 ?
Ag2 C7 2.248(17) 3_565 ?
Ag2 C7A 2.57(3) . ?
Ag2 C7A 2.57(3) 3_565 ?
Ag2 C7A 2.57(3) 2_665 ?
C1 C2 1.183(9) . ?
C1 Ag3 2.360(7) 3_565 ?
C1 Ag3 2.406(7) 14_456 ?
C1 Ag3A 2.428(8) 14_456 ?
C1 Ag3A 2.534(8) 3_565 ?
C2 C3 1.476(11) . ?
C3 C4 1.529(10) . ?
C3 C5 1.513(9) . ?
C3 C6 1.542(10) . ?
C3 C4A 1.538(10) . ?
C3 C5A 1.541(9) . ?
C3 C6A 1.502(9) . ?
Ag3 C7 2.495(18) . ?
C4 H4A 0.9597 . ?
C4 H4B 0.9604 . ?
C4 H4C 0.9600 . ?
C5 H5A 0.9601 . ?
C5 H5B 0.9600 . ?
C5 H5C 0.9596 . ?
C6 H6A 0.9602 . ?
C6 H6B 0.9602 . ?
C6 H6C 0.9597 . ?
C7 C8 1.19(2) . ?
C8 C9 1.503(15) . ?
C9 C10 1.533(10) . ?
C9 C11 1.526(10) . ?
C9 C12 1.530(10) . ?
C10 H10A 0.9800 . ?
C10 H10B 0.9800 . ?
C10 H10C 0.9800 . ?
C11 H11A 0.9800 . ?
C11 H11B 0.9800 . ?
C11 H11C 0.9800 . ?
C12 H12A 0.9800 . ?
C12 H12B 0.9800 . ?
C12 H12C 0.9800 . ?
Ag3A C7A 2.13(3) . ?
Ag3A C8A 2.54(2) . ?
C4A H4AA 0.9597 . ?
C4A H4AB 0.9600 . ?
C4A H4AC 0.9603 . ?
C5A H5AA 0.9800 . ?
C5A H5AB 0.9800 . ?
C5A H5AC 0.9800 . ?
C6A H6AA 0.9800 . ?
C6A H6AB 0.9800 . ?
C6A H6AC 0.9800 . ?
C7A C8A 1.16(4) . ?
C8A C9A 1.467(18) . ?
C9A C10A 1.526(10) . ?
C9A C11A 1.526(10) . ?
C9A C12A 1.526(10) . ?
C10A H10D 0.9603 . ?
C10A H10E 0.9597 . ?
C10A H10F 0.9604 . ?
C11A H11D 0.9598 . ?
C11A H11E 0.9601 . ?
C11A H11F 0.9605 . ?
C12A H12D 0.9800 . ?
C12A H12E 0.9800 . ?
C12A H12F 0.9800 . ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Ag1 C7A C8A Ag3A -122(7) . . . . ?
Ag2 C7A C8A Ag3A 115(3) . . . . ?
Ag3A C8A C9A C10A -14(3) . . . . ?
Ag3A C8A C9A C11A 102(2) . . . . ?
Ag3A C8A C9A C12A -135(2) . . . . ?
loop_
_smtbx_masks_void_nr
_smtbx_masks_void_average_x
_smtbx_masks_void_average_y
_smtbx_masks_void_average_z
_smtbx_masks_void_volume
_smtbx_masks_void_count_electrons
_smtbx_masks_void_content
1 0.000 0.000 0.257 7.8 1.1 ?
2 0.000 0.000 0.500 245.0 72.7 '0.333 C10O13H43'
3 0.000 0.000 0.743 7.8 0.0 ?
4 0.333 0.667 0.167 245.0 72.6 '0.333 C10O13H43'
5 -0.333 0.333 0.833 245.0 72.6 '0.333 C10O13H43'
6 0.333 0.667 0.410 7.8 0.0 ?
7 0.333 0.667 0.923 7.8 1.1 ?
8 0.667 0.333 0.077 7.8 0.0 ?
9 0.667 0.333 0.590 7.8 1.1 ?
